# Crystal Structure Determination II - Khwarizmi Science Society

date post

03-Feb-2022Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Crystal Structure Determination II - Khwarizmi Science Society

Slide 109/10/2010

Diffraction Intensities

The integrated intensity, I (hkl) (peak area) of each powder diffraction peak with miller indices, hkl, is given by the following expression:

I (hkl) = |F|2 × Mhkl × LP (θ) × TF (θ) × A (θ)

where

LP (θ) = Lorentz and Polarization factors

TF (θ) = Temperature Factor (more correctly referred to as the displacement parameter)

A (θ) = Absorption Factor

This does not include effects that can sometimes by problematic such as preferred orientation and extinction.

Multiplicity Factor

In a powder diffraction experiment the d-spacings for related reflections are often equivalent. Consider the examples below:

Cubic

– (100), (010), (001), (-100), (0-10), (00-1) → Equivalent Multiplicity Factor = 6

– (110), (-110), (1-10), (-1-10), (101), (-101), (10-1), (-10-1), (011), (0-11), (01-1), (0-1-1) → Equivalent Multiplicity Factor = 12

In general for a cubic system where the Miller indices are n1, n2 and n3 (all unequal) the multiplicity factors Mhkl are:

n100 (i.e. 100) → M = 6 n1n1n1 (ie 111) → M = 8 n1n10 (i.e. 110) → M = 12 n1n20 (ie 210) → M = 24 n1n1n2 (i.e. 221) → M = 24 n1n2n3 (ie 321) → M = 48

The multiplicities are lower in lower symmetry systems. For example in a tetragonal crystal the (100) is equivalent with the (010), (-100) and (0-10), but not with the (001) and the (00-1).

Multiplicity Factor

System hkl hhl hh0 0kk hhh hk0 h0l 0kl h00 0k0 00l

Cubic 48 24 12 12 8 24 24 24 6 6 6

Tetragonal 16 8 4 8 8 8 8 8 4 4 2

Hexagonal 24 12 6 12 12 12 12 12 6 6 2

Orthorhombic 8 8 8 8 8 4 4 4 2 2 2

Monoclinic 4 4 4 4 4 4 2 4 2 2 2

Triclinic 2 2 2 2 2 2 2 2 2 2 2

Scattering by an Atom We can consider an atom to be a collection of electrons. The electrons around an atom scatter radiation in the manner described by Thompson. However, due to the coherence of the radiation we need to consider interference effects from different electrons within an atom. This leads to a strong anglular dependence of the scattering. A quantity f, the atomic scattering factor, is used to describe the efficiency of scattering of a given atom in a given direction. It is defined as a ratio of amplitudes:

amplitude of the wave scattered by an atom f = ———————————————————————

amplitude of the wave scattered by one electron

For any atom scattering in the forward direction f is equal to its atomic number Z, f = Z. As θ increases, the waves scattered by individual electrons become more and more out of phase and f decreases. The atomic scattering factor also depends on the wavelength of the incident beam: at fixed value of θ, f will be smaller with the shorter wavelength, since the path differences will be larger relative to the wavelength, leading to greater interferences between the scattered beams.

The actual calculation of f involves sinθ rather than θ, so that the net effect is that f decreases as the quantity (sinθ/λ) increases. The scattering factor is some times called the form factor, because it depends on the way in which the electrons are distributed around the nucleus.

Structure Factor The structure factor reflects the interference between atoms in the unit cell. All of the information regarding where the atoms are located in the unit cell is contained in the structure factor. The structure factor is given by the following summation over all atoms in the unit cell.

The value of this function is 1 for even multiples of 2π and -1 for odd multiples of 2π.

Structure Factor Calculations 1. Base-centered unit cell. Two atoms of the same kind located at 0 0 0 and 1/2 1/2 0

F = f e2π i (0) + f e2π i (h/2 + k/2)

= f (1 + eπ i (h + k) )

= 2f for h and k unmixed (both even or both odd)

= 0 for h and k mixed (one even and one odd)

The value of l index has no effect on the structure factor

Hence 111, 112, 113 all have the same value of F

2. Body-centered unit cell. Two atoms of the same kind located

at 0 0 0 and 1/2 1/2 1/2.

F = f e2π i (0) + f e2π i (h/2 + k/2 + l/2)

= f (1 + eπ i (h + k + l) )

= 2f when (h + k + l) is even

= 0 when (h + k + l) is odd

3. Face-centered unit cell. Four atoms of the same kind located at 0 0 0, 1/2 1/2 0, 1/2 0 1/2 and 0 1/2 1/2. F = f e2π i (0) + f e2π i (h/2 + k/2) + f e2π i (h/2 + l/2) + f e2π i (k/2 + l/2)

= f [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] If h, k, and l are unmixed, then the sums (h + k), (h + l) and (k + l) are even integers and each term in the above equation has the value 1. F = 4f for unmixed indices; If h, k and l are mixed, then the sum of the three exponentials is -1, whether two of the indices are odd and one even or two even and one odd. So F = 0 for mixed indices Thus, reflections may occur for such planes as (111), (200) and (220) but not for the planes (100), (210), (112) etc.

Note: Structure factor is independent of the shape and size of the unit cell. It means that rules of missing reflections apply to all kinds of unit cells of any dimension; cubic, tetragonal, orthorhombic etc.

4. The Example of NaCl: It has a cubic lattice with 4 Na and 4 Cl atoms per unit cell, located as follows: Na 0 0 0 1/2 1/2 0 1/2 0 1/2 0 1/2 1/2 Cl 1/2 1/2 1/2 1/2 0 0 0 1/2 0 0 0 1/2

F = fNa e2π i (0) + fNa e2π i (h/2 + k/2) + fNa e2π i (h/2 + l/2) + fNa e2π i (k/2 + l/2) + fCl e2π i (h/2 + k/2 + l/2) +

fCl e2π i (h/2) + fCl e2π i (k/2) + fCl e2π i ( l/2)

= fNa [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] + fCl [eπ i (h + k + l) + eπ ih + eπ ik + eπ il ]

In case of NaCl, the sodium-atom positions are related by the face centering translations and so are the chlorine-atom positions. Whenever a lattice contains common translations, the corresponding terms in the structure factor equation can always be factored out, leading to considerable simplification. In this case:

F = fNa [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] + fCl eπ i (h + k + l) [1 + eπ i (−k − l) + eπ i (−h − l) + eπ i (−h − k) ]

The signs of the exponents in the second bracket may be changed:

F = fNa [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] + fCl eπ i (h + k + l) [1 + eπ i (k + l) + eπ i (h + l) + eπ i (h + k) ]

As enπi = e−nπ i

F = [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] [ fNa + fCl eπ i (h + k + l) ]

Here the terms corresponding to the face-centering translations appear in the first factor; the second term contains the terms that describe the “basis” of the unit cell, namely, the Na atom at 0 0 0 and the Cl atom at ½ ½ ½. The first term have a total value of zero for mixed indices and 4 for unmixed indices as described earlier for face-cetered unit cell. This shows at once that NaCl has a face-centered lattice and that:

F = 0 for mixed indices

F2 = 0

F = 4 (fNa + fCl ) if (h + k + l) is even;

F2 = 16 (fNa + fCl )2

F = 4 (fNa − fCl ) if (h + k + l) is odd;

F2 = 16 (fNa − fCl )2

In this case , there are more than four atoms per unit cell (8), but the lattice is still face-

centered. The introduction of additional atoms has not eliminated any reflections present

in the case of the four-atom cell, but it has decreased some in intensity.

5. Example CsCl

• Let’s calculate the structure factors for the first 6 peaks of CsCl. To do this we need to know the atomic positions and the Miller Indices.

F = fCl e2π i (0) + fCs e2π i (h/2 + k/2 + l/2)

F = fCl e2π i (0) + fCs eπ i (h + k + l)

F = fCl − fCs when (h + k + l) is odd number

F = fCl + fCs when (h + k + l) is even number

F100 = fCl − fCs F110 = fCl + fCs

F111 = fCl − fCs F220 = fCl + fCs

F210 = fCl − fCs F221 = fCl + fCs

Temperature Factor

The atoms in a crystal undergo thermal vibration about their mean positions and the amplitude of this vibration increases as the temperature is increased. For example at room temperature the average displacement of an atom of aluminum from its mean position is 0.17 Å, which is about 6 percent of the distance of closest approach of the mean atom positions in this crystal.

Thermal vibration of the atoms has three main effects:

1. The unit cell expands, causing changes in periodicity of d and therefore in the 2θ positions of the diffraction lines.

2. The intensities of the diffraction lines decrease 3. The intensity of the background scattering between lines increases.

Thermal agitation decreases the intensity of diffracted beam because it degrades the periodicity of the lattice. In intensity calculations this effect is included by introducing the temperature factor e−2M, which is a number by which the calculated intensity is to be multiplied to allow for thermal vibration of the atoms. (f = f0 e−M)

The quantity M depends on both the amplitude of thermal vibration and the scattering angle 2θ.

M = 8π2 2 (sinθ/ λ)2 = B (sinθ/λ )2

Where is the mean square displacement of the atom in a direction normal to the diffracting plane and the coefficient B is the isotropic temperature factor and is proportional to the mean squared displacement of the atoms.

More sophisticated treatments assume different values of B for each crystallographically independent atom and anisotropic vibrations (elliptical in shape rather than spherical).

Isotropic factor: B or

Anisotropic factor: B11, B22, B33, B12, B13, B23, 11, 22, 33, 12, 13, 23

The thermal vibration of atoms has another effect on diffraction patterns. Besides decreasing the intensity of diffraction lines, it causes some general coherent scattering in all directions. This is called temperature-diffuse scattering; it contributes only to the general background of the pattern and its intensity gradually increases with 2θ.

Absorption Factor

According to Beer’s law, absorption reduces the intensity of an X-ray beam travelling through a given material by an amount which depends on the material and the length of the path travelled by the radiation in it.

The intensity of the diffracted X-rays is reduced due to absorption by the factor:

I /I0 = e−µx

Here x is the total path length and µ is the linear absorption coefficient of the crystal.

Lorentz Factor There are a number of factors that lead to angle dependence of the peak intensities (integrated intensities).

1. Diffraction can occur for angles slightly different from the value predicted by Bragg’s Law → I ∝ 1/sin(2θ).

2. The number of crystals oriented in such a way as to satisfy Bragg’s Law is highest for low angles → I ∝ cos(θ)

3. The fraction of the diffraction cone that intersects the detector is highest at low angles → I ∝ 1/sin(2θ)

When combine these considerations and do some trigonometric manipulation we get the Lorentz Factor:

I ∝ 1/(4sin2θ cosθ)

Polarization and the LP Factor An X-ray propagating in the x-direction will have an electric vector oriented in the yz plane. The y and z components of the X-ray will be scattered differently because the angle between the scattered beam and the electric field gradient will differ, as derived by Thompson. This leads to the polarization factor:

I ∝ (1+cos22θ)/2

Typically the Lorentz and Polarization terms are combined to give the Lorentz- Polarization (LP) factor.

I ∝ (1+cos22θ)/(8sin2θ cosθ)

The overall effect of these geometrical factors is to decrease the intensity of the reflections at intermediate angle compared to those in forward or backward directions.

Extinctions

Intensity calculation formula is derived for “ideally imperfect” crystal, one consisting of quite small mosaic blocks which are randomly oriented. Such a crystal has maximum diffracting power. A crystal made up of large mosaic blocks is more nearly perfect and has a lower diffracting power. This decrease in the integrated intensity of the diffracted beam as the crystal becomes more nearly perfect is called extinction. Destructive interference from re-reflections within the crystals. The strong peaks appear weaker. The solution is to grind the powdered sample more.

Examples of Intensity Calculation 1. Peak Positions and Intensity Calculations for copper Copper is an face-centered cubic with cell parameter a = 3.615 Å. Diffraction pattern is measured with Cu Kα radiation.

1 2 3 4 5 6 7 8

Line hkl h2 +k2+l2 sin2θ sinθ θ sinθ /λ fcu

1 111 3 0.1365 0.369 21.7 0.24 22.1

2 200 4 0.1820 0.427 25.3 0.27 20.9

3 220 8 0.364 0.603 37.1 0.39 16.8

4 311 11 0.500 0.707 45.0 0.46 14.8

5 222 12 0.546 0.739 47.6 0.48 14.2

6 400 16 0.728 0.853 58.5 0.55 12.5

7 331 19 0.865 0.930 68.4 0.60 11.5

8 420 20 0.910 0.954 72.6 0.62 11.1

1 9 10 11 12 13 14

Line F2 M LP Cal. Intensity Relative Intensity (%)

Obs. Intensity

2. Peak Positions and Intensity Calculations ZnS

ZnS (zinc blende) is cubic and has a lattice parameter of 5.41 Å.

The first step is to calculate the structure factor. ZnS has four zinc and four sulfur atoms per unit cell, located at the following positions.

Zn: ¼ ¼ ¼ + face-centering translations S: 0 0 0 + face-centering translations

Since structure is face-centered, the structure factor will be zero for planes of mixed indices. From example of NaCl, the terms in the structure factor equation corresponding to the face-centering translations can be factored out and the equation for unmixed indices written down at once:

F = 4[fs + fZn e(πi/2)(h + k + l)]

|F|2 is obtained by multiplication of the above by its complex conjugate:

|F|2 = 16[fs + fZn e(πi/2)(h + k + l)] [fs + fZn e−(πi/2)(h + k + l)]

This reduces to the following form:

|F|2 = 16[f2 s + f2

Zn +2fsfZn cos(x/2)(h + k + l)]

Further simplification is possible for various special cases:

|F|2 = 16[f2 s + f2

Zn ] when (h + k + l) is odd

|F|2 = 16[fs − fZn ]2 when (h + k + l) is an odd multiple of 2

|F|2 = 16[fs + fZn ]2 when (h + k + l) is an even multiple of 2

The intensity calculations are carried out in the table below:

1 2 3 4 5 6

Line hkl θ sinθ /λ fS fZn

1 111 14.3 0.16 12.3 25.8

2 200 16.6 0.19 11.4 24.6

3 220 23.8 0.26 9.7 22.1

4 311 28.2 0.30 9.0 20.7

5 222 29.6 0.32 8.8 20.0

6 400 34.8 0.37 8.2 18.4

1 7 8 9 10 11

Line F2 M LP Relative Intensity (%) (Calc.)

Obs. Intensity

Determination of Atom Positions

The observed relative intensities are determined by the atom positions in the unit cell. However, there is no known procedure of directly calculating atom positions from observed intensities.

Atom positions are rather calculated by trial and error method. A set of atom positions is assumed, the intensities corresponding to these positions are calculated and the calculated intensities are compared with the observed ones, the process being repeated until satisfactory agreement is reached. This trial method is further aided by the accumulated knowledge of previously known structures. From these known structures a few likely candidates may be selected as a starting point.

There are many complex structures which can not be solved by this simple approach. Two powerful methods of space group theory and Fourier series are used in these cases. For example if a given substance is known to be tetragonal and to have n atoms in its unit cell, then space-group theory lists all possible arrangements of n atoms which will have tetragonal symmetry. This listing of possible arrangements is further aided by the knowledge of systematic absences.

A Fourier series is a type of infinite trigonometric series by which any kind of periodic function may be expressed. Now the one essential property of a crystal is that its atoms are arranged in space in a periodic fashion. This means that density of electrons is also a periodic function of position in the crystal, rising to maximum at the point where an atom is located and dropping to a low value in the region between atoms. Since the electron density is a periodic function of position of atoms, a crystal may be described analytically by means of the Fourier series.

Example of Structure Determination

Consider an intermediate phase which occurs in the cadmium-tellurium system. Chemical analysis of the specimen showed that it contains 46.6 weight percent Cd and 53.4 weight percent Te. This is equivalent to 49.8 atomic percent Cd and can be represented by the formula CdTe. Powder X-ray diffraction pattern was collected by using Cu Kα radiation.

The observed values of sin2θ for the first 16 lines are listed in the Table 1, together with the visually estimated relative line intensities. This pattern can be indexed on the basis of a cubic unit cell and the indices of the observed lines are given in the Table 1. The lattice parameter, calculated from the sin2θ value for the highest line, is 6.46 Å.

The density of the specimen, as determined by weighing a quantity of the powder in a pyknometer bottle was 5.82 g/cm3.

The sum of atomic weights can be calculated as:

945 66042.1

)46.6)(82.5( 3

==∑ A

Since the molecular weight of CdTe is 240.02, the number of molecules per unit cell is 945/240.02 = 3.94, or 4 within experimental error.

Knowing the unit cell of CdTe is cubic and that it contains 4 molecules of CdTe, i.e., 4 atoms of Cd and 4 atoms of Te, possible arrangement of these atoms in the unit cell can be evaluated.

Examination of the indices listed in Table 1 reveals that the indices of the observed lines are all unmixed and that the…

Diffraction Intensities

The integrated intensity, I (hkl) (peak area) of each powder diffraction peak with miller indices, hkl, is given by the following expression:

I (hkl) = |F|2 × Mhkl × LP (θ) × TF (θ) × A (θ)

where

LP (θ) = Lorentz and Polarization factors

TF (θ) = Temperature Factor (more correctly referred to as the displacement parameter)

A (θ) = Absorption Factor

This does not include effects that can sometimes by problematic such as preferred orientation and extinction.

Multiplicity Factor

In a powder diffraction experiment the d-spacings for related reflections are often equivalent. Consider the examples below:

Cubic

– (100), (010), (001), (-100), (0-10), (00-1) → Equivalent Multiplicity Factor = 6

– (110), (-110), (1-10), (-1-10), (101), (-101), (10-1), (-10-1), (011), (0-11), (01-1), (0-1-1) → Equivalent Multiplicity Factor = 12

In general for a cubic system where the Miller indices are n1, n2 and n3 (all unequal) the multiplicity factors Mhkl are:

n100 (i.e. 100) → M = 6 n1n1n1 (ie 111) → M = 8 n1n10 (i.e. 110) → M = 12 n1n20 (ie 210) → M = 24 n1n1n2 (i.e. 221) → M = 24 n1n2n3 (ie 321) → M = 48

The multiplicities are lower in lower symmetry systems. For example in a tetragonal crystal the (100) is equivalent with the (010), (-100) and (0-10), but not with the (001) and the (00-1).

Multiplicity Factor

System hkl hhl hh0 0kk hhh hk0 h0l 0kl h00 0k0 00l

Cubic 48 24 12 12 8 24 24 24 6 6 6

Tetragonal 16 8 4 8 8 8 8 8 4 4 2

Hexagonal 24 12 6 12 12 12 12 12 6 6 2

Orthorhombic 8 8 8 8 8 4 4 4 2 2 2

Monoclinic 4 4 4 4 4 4 2 4 2 2 2

Triclinic 2 2 2 2 2 2 2 2 2 2 2

Scattering by an Atom We can consider an atom to be a collection of electrons. The electrons around an atom scatter radiation in the manner described by Thompson. However, due to the coherence of the radiation we need to consider interference effects from different electrons within an atom. This leads to a strong anglular dependence of the scattering. A quantity f, the atomic scattering factor, is used to describe the efficiency of scattering of a given atom in a given direction. It is defined as a ratio of amplitudes:

amplitude of the wave scattered by an atom f = ———————————————————————

amplitude of the wave scattered by one electron

For any atom scattering in the forward direction f is equal to its atomic number Z, f = Z. As θ increases, the waves scattered by individual electrons become more and more out of phase and f decreases. The atomic scattering factor also depends on the wavelength of the incident beam: at fixed value of θ, f will be smaller with the shorter wavelength, since the path differences will be larger relative to the wavelength, leading to greater interferences between the scattered beams.

The actual calculation of f involves sinθ rather than θ, so that the net effect is that f decreases as the quantity (sinθ/λ) increases. The scattering factor is some times called the form factor, because it depends on the way in which the electrons are distributed around the nucleus.

Structure Factor The structure factor reflects the interference between atoms in the unit cell. All of the information regarding where the atoms are located in the unit cell is contained in the structure factor. The structure factor is given by the following summation over all atoms in the unit cell.

The value of this function is 1 for even multiples of 2π and -1 for odd multiples of 2π.

Structure Factor Calculations 1. Base-centered unit cell. Two atoms of the same kind located at 0 0 0 and 1/2 1/2 0

F = f e2π i (0) + f e2π i (h/2 + k/2)

= f (1 + eπ i (h + k) )

= 2f for h and k unmixed (both even or both odd)

= 0 for h and k mixed (one even and one odd)

The value of l index has no effect on the structure factor

Hence 111, 112, 113 all have the same value of F

2. Body-centered unit cell. Two atoms of the same kind located

at 0 0 0 and 1/2 1/2 1/2.

F = f e2π i (0) + f e2π i (h/2 + k/2 + l/2)

= f (1 + eπ i (h + k + l) )

= 2f when (h + k + l) is even

= 0 when (h + k + l) is odd

3. Face-centered unit cell. Four atoms of the same kind located at 0 0 0, 1/2 1/2 0, 1/2 0 1/2 and 0 1/2 1/2. F = f e2π i (0) + f e2π i (h/2 + k/2) + f e2π i (h/2 + l/2) + f e2π i (k/2 + l/2)

= f [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] If h, k, and l are unmixed, then the sums (h + k), (h + l) and (k + l) are even integers and each term in the above equation has the value 1. F = 4f for unmixed indices; If h, k and l are mixed, then the sum of the three exponentials is -1, whether two of the indices are odd and one even or two even and one odd. So F = 0 for mixed indices Thus, reflections may occur for such planes as (111), (200) and (220) but not for the planes (100), (210), (112) etc.

Note: Structure factor is independent of the shape and size of the unit cell. It means that rules of missing reflections apply to all kinds of unit cells of any dimension; cubic, tetragonal, orthorhombic etc.

4. The Example of NaCl: It has a cubic lattice with 4 Na and 4 Cl atoms per unit cell, located as follows: Na 0 0 0 1/2 1/2 0 1/2 0 1/2 0 1/2 1/2 Cl 1/2 1/2 1/2 1/2 0 0 0 1/2 0 0 0 1/2

F = fNa e2π i (0) + fNa e2π i (h/2 + k/2) + fNa e2π i (h/2 + l/2) + fNa e2π i (k/2 + l/2) + fCl e2π i (h/2 + k/2 + l/2) +

fCl e2π i (h/2) + fCl e2π i (k/2) + fCl e2π i ( l/2)

= fNa [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] + fCl [eπ i (h + k + l) + eπ ih + eπ ik + eπ il ]

In case of NaCl, the sodium-atom positions are related by the face centering translations and so are the chlorine-atom positions. Whenever a lattice contains common translations, the corresponding terms in the structure factor equation can always be factored out, leading to considerable simplification. In this case:

F = fNa [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] + fCl eπ i (h + k + l) [1 + eπ i (−k − l) + eπ i (−h − l) + eπ i (−h − k) ]

The signs of the exponents in the second bracket may be changed:

F = fNa [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] + fCl eπ i (h + k + l) [1 + eπ i (k + l) + eπ i (h + l) + eπ i (h + k) ]

As enπi = e−nπ i

F = [1 + eπ i (h + k) + eπ i (h + l) + eπ i (k + l) ] [ fNa + fCl eπ i (h + k + l) ]

Here the terms corresponding to the face-centering translations appear in the first factor; the second term contains the terms that describe the “basis” of the unit cell, namely, the Na atom at 0 0 0 and the Cl atom at ½ ½ ½. The first term have a total value of zero for mixed indices and 4 for unmixed indices as described earlier for face-cetered unit cell. This shows at once that NaCl has a face-centered lattice and that:

F = 0 for mixed indices

F2 = 0

F = 4 (fNa + fCl ) if (h + k + l) is even;

F2 = 16 (fNa + fCl )2

F = 4 (fNa − fCl ) if (h + k + l) is odd;

F2 = 16 (fNa − fCl )2

In this case , there are more than four atoms per unit cell (8), but the lattice is still face-

centered. The introduction of additional atoms has not eliminated any reflections present

in the case of the four-atom cell, but it has decreased some in intensity.

5. Example CsCl

• Let’s calculate the structure factors for the first 6 peaks of CsCl. To do this we need to know the atomic positions and the Miller Indices.

F = fCl e2π i (0) + fCs e2π i (h/2 + k/2 + l/2)

F = fCl e2π i (0) + fCs eπ i (h + k + l)

F = fCl − fCs when (h + k + l) is odd number

F = fCl + fCs when (h + k + l) is even number

F100 = fCl − fCs F110 = fCl + fCs

F111 = fCl − fCs F220 = fCl + fCs

F210 = fCl − fCs F221 = fCl + fCs

Temperature Factor

The atoms in a crystal undergo thermal vibration about their mean positions and the amplitude of this vibration increases as the temperature is increased. For example at room temperature the average displacement of an atom of aluminum from its mean position is 0.17 Å, which is about 6 percent of the distance of closest approach of the mean atom positions in this crystal.

Thermal vibration of the atoms has three main effects:

1. The unit cell expands, causing changes in periodicity of d and therefore in the 2θ positions of the diffraction lines.

2. The intensities of the diffraction lines decrease 3. The intensity of the background scattering between lines increases.

Thermal agitation decreases the intensity of diffracted beam because it degrades the periodicity of the lattice. In intensity calculations this effect is included by introducing the temperature factor e−2M, which is a number by which the calculated intensity is to be multiplied to allow for thermal vibration of the atoms. (f = f0 e−M)

The quantity M depends on both the amplitude of thermal vibration and the scattering angle 2θ.

M = 8π2 2 (sinθ/ λ)2 = B (sinθ/λ )2

Where is the mean square displacement of the atom in a direction normal to the diffracting plane and the coefficient B is the isotropic temperature factor and is proportional to the mean squared displacement of the atoms.

More sophisticated treatments assume different values of B for each crystallographically independent atom and anisotropic vibrations (elliptical in shape rather than spherical).

Isotropic factor: B or

Anisotropic factor: B11, B22, B33, B12, B13, B23, 11, 22, 33, 12, 13, 23

The thermal vibration of atoms has another effect on diffraction patterns. Besides decreasing the intensity of diffraction lines, it causes some general coherent scattering in all directions. This is called temperature-diffuse scattering; it contributes only to the general background of the pattern and its intensity gradually increases with 2θ.

Absorption Factor

According to Beer’s law, absorption reduces the intensity of an X-ray beam travelling through a given material by an amount which depends on the material and the length of the path travelled by the radiation in it.

The intensity of the diffracted X-rays is reduced due to absorption by the factor:

I /I0 = e−µx

Here x is the total path length and µ is the linear absorption coefficient of the crystal.

Lorentz Factor There are a number of factors that lead to angle dependence of the peak intensities (integrated intensities).

1. Diffraction can occur for angles slightly different from the value predicted by Bragg’s Law → I ∝ 1/sin(2θ).

2. The number of crystals oriented in such a way as to satisfy Bragg’s Law is highest for low angles → I ∝ cos(θ)

3. The fraction of the diffraction cone that intersects the detector is highest at low angles → I ∝ 1/sin(2θ)

When combine these considerations and do some trigonometric manipulation we get the Lorentz Factor:

I ∝ 1/(4sin2θ cosθ)

Polarization and the LP Factor An X-ray propagating in the x-direction will have an electric vector oriented in the yz plane. The y and z components of the X-ray will be scattered differently because the angle between the scattered beam and the electric field gradient will differ, as derived by Thompson. This leads to the polarization factor:

I ∝ (1+cos22θ)/2

Typically the Lorentz and Polarization terms are combined to give the Lorentz- Polarization (LP) factor.

I ∝ (1+cos22θ)/(8sin2θ cosθ)

The overall effect of these geometrical factors is to decrease the intensity of the reflections at intermediate angle compared to those in forward or backward directions.

Extinctions

Intensity calculation formula is derived for “ideally imperfect” crystal, one consisting of quite small mosaic blocks which are randomly oriented. Such a crystal has maximum diffracting power. A crystal made up of large mosaic blocks is more nearly perfect and has a lower diffracting power. This decrease in the integrated intensity of the diffracted beam as the crystal becomes more nearly perfect is called extinction. Destructive interference from re-reflections within the crystals. The strong peaks appear weaker. The solution is to grind the powdered sample more.

Examples of Intensity Calculation 1. Peak Positions and Intensity Calculations for copper Copper is an face-centered cubic with cell parameter a = 3.615 Å. Diffraction pattern is measured with Cu Kα radiation.

1 2 3 4 5 6 7 8

Line hkl h2 +k2+l2 sin2θ sinθ θ sinθ /λ fcu

1 111 3 0.1365 0.369 21.7 0.24 22.1

2 200 4 0.1820 0.427 25.3 0.27 20.9

3 220 8 0.364 0.603 37.1 0.39 16.8

4 311 11 0.500 0.707 45.0 0.46 14.8

5 222 12 0.546 0.739 47.6 0.48 14.2

6 400 16 0.728 0.853 58.5 0.55 12.5

7 331 19 0.865 0.930 68.4 0.60 11.5

8 420 20 0.910 0.954 72.6 0.62 11.1

1 9 10 11 12 13 14

Line F2 M LP Cal. Intensity Relative Intensity (%)

Obs. Intensity

2. Peak Positions and Intensity Calculations ZnS

ZnS (zinc blende) is cubic and has a lattice parameter of 5.41 Å.

The first step is to calculate the structure factor. ZnS has four zinc and four sulfur atoms per unit cell, located at the following positions.

Zn: ¼ ¼ ¼ + face-centering translations S: 0 0 0 + face-centering translations

Since structure is face-centered, the structure factor will be zero for planes of mixed indices. From example of NaCl, the terms in the structure factor equation corresponding to the face-centering translations can be factored out and the equation for unmixed indices written down at once:

F = 4[fs + fZn e(πi/2)(h + k + l)]

|F|2 is obtained by multiplication of the above by its complex conjugate:

|F|2 = 16[fs + fZn e(πi/2)(h + k + l)] [fs + fZn e−(πi/2)(h + k + l)]

This reduces to the following form:

|F|2 = 16[f2 s + f2

Zn +2fsfZn cos(x/2)(h + k + l)]

Further simplification is possible for various special cases:

|F|2 = 16[f2 s + f2

Zn ] when (h + k + l) is odd

|F|2 = 16[fs − fZn ]2 when (h + k + l) is an odd multiple of 2

|F|2 = 16[fs + fZn ]2 when (h + k + l) is an even multiple of 2

The intensity calculations are carried out in the table below:

1 2 3 4 5 6

Line hkl θ sinθ /λ fS fZn

1 111 14.3 0.16 12.3 25.8

2 200 16.6 0.19 11.4 24.6

3 220 23.8 0.26 9.7 22.1

4 311 28.2 0.30 9.0 20.7

5 222 29.6 0.32 8.8 20.0

6 400 34.8 0.37 8.2 18.4

1 7 8 9 10 11

Line F2 M LP Relative Intensity (%) (Calc.)

Obs. Intensity

Determination of Atom Positions

The observed relative intensities are determined by the atom positions in the unit cell. However, there is no known procedure of directly calculating atom positions from observed intensities.

Atom positions are rather calculated by trial and error method. A set of atom positions is assumed, the intensities corresponding to these positions are calculated and the calculated intensities are compared with the observed ones, the process being repeated until satisfactory agreement is reached. This trial method is further aided by the accumulated knowledge of previously known structures. From these known structures a few likely candidates may be selected as a starting point.

There are many complex structures which can not be solved by this simple approach. Two powerful methods of space group theory and Fourier series are used in these cases. For example if a given substance is known to be tetragonal and to have n atoms in its unit cell, then space-group theory lists all possible arrangements of n atoms which will have tetragonal symmetry. This listing of possible arrangements is further aided by the knowledge of systematic absences.

A Fourier series is a type of infinite trigonometric series by which any kind of periodic function may be expressed. Now the one essential property of a crystal is that its atoms are arranged in space in a periodic fashion. This means that density of electrons is also a periodic function of position in the crystal, rising to maximum at the point where an atom is located and dropping to a low value in the region between atoms. Since the electron density is a periodic function of position of atoms, a crystal may be described analytically by means of the Fourier series.

Example of Structure Determination

Consider an intermediate phase which occurs in the cadmium-tellurium system. Chemical analysis of the specimen showed that it contains 46.6 weight percent Cd and 53.4 weight percent Te. This is equivalent to 49.8 atomic percent Cd and can be represented by the formula CdTe. Powder X-ray diffraction pattern was collected by using Cu Kα radiation.

The observed values of sin2θ for the first 16 lines are listed in the Table 1, together with the visually estimated relative line intensities. This pattern can be indexed on the basis of a cubic unit cell and the indices of the observed lines are given in the Table 1. The lattice parameter, calculated from the sin2θ value for the highest line, is 6.46 Å.

The density of the specimen, as determined by weighing a quantity of the powder in a pyknometer bottle was 5.82 g/cm3.

The sum of atomic weights can be calculated as:

945 66042.1

)46.6)(82.5( 3

==∑ A

Since the molecular weight of CdTe is 240.02, the number of molecules per unit cell is 945/240.02 = 3.94, or 4 within experimental error.

Knowing the unit cell of CdTe is cubic and that it contains 4 molecules of CdTe, i.e., 4 atoms of Cd and 4 atoms of Te, possible arrangement of these atoms in the unit cell can be evaluated.

Examination of the indices listed in Table 1 reveals that the indices of the observed lines are all unmixed and that the…